1 Per. Mineral. (1999), 68, 1, 1-11 [';\] PERIODICO di MINERALOGIA established in 1930 An Intemational Journal of MINERALOGY, CRYSTALLOGRAPHY, GEOCHEMISTRY, ORE DEPOSITS, PETROLOGY, VOLCANOLOGY and applied topics on Environment, Archaeometry and Cultural Heritage The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials ALESSANDRO F. GUALTIERI* Dipartimento di Scienze della Terra, Universita di Modena e Reggio Emilia, ViaS. Eufemia 19, Modena, Italy Submitted, January Accepted, Februmy 1999 ABSTRACT. - Fibrous asbestos minerals have been identified as priority substances for risk reduction and pollution prevention. Because of the well known hazardous effects associated with past occupational exposures to asbestos and because of its widespread use in commerce, exposures to asbestos present a general health hazard. Therefore, the identification and quantification of asbestos in bulk materials which are still sited in a number of plants and public buildings is fundamental for a proper plan of social prevention and general intervention. X-ray powder diffraction is considered an effective tool of investigation of bulk materials with a high statistical significance. The combined Rietveld-RIR method, has been successfully applied for the quantitative determination in the past of asbestos in bulk materials such as insulating cements, mixed asbestos-slag wools, contaminated soils, and others. The University of Jussieu in Paris has been partly evacuated because the framework of the building is composed of an asbestos rich material. This paper reports the description of the characterisation of that material and a possible plan of intervention for the treatment of the hazardous material in situ. RIASSUNTO. - E noto gia da parecchio tempo che i materiali fibrosi classificati genericamente come *Phone: , fax: , asbesti (appartenenti alia famiglia del serpentino nella varieta crisotilo ed alia famiglia dell'anfibolo varieta riebeckite e grunerite) sono potenziali agenti cancerogeni. Data la presenza a tutt' oggi sui territorio di milioni di m2 di prodotti quali il cementoamianto o I' ami an to fioccato contenenti percentuali variabili da 0.5 a 20% in peso di asbesto, la caratterizzazione di questi materiali per una corretta classificazione e trattamento, e condizione essenziale per qualsiasi tipo di intervento. La diffrazione di raggi X su polveri si e dimostrata, ancora una volta, strumento fondamentale per la caratterizzazione in bulk dei materiali. La tecnica che ven a descritta si avvale della combinazione del metodo Rietveld e del metodo RIR (Reference Intensity Ratio) per arrivare alia determinazione quantitativa di asbesto in materiali massivi contenenti fibre di Iana di vetro (materiale amorfo). Nel presente lavoro viene descritta in particolare I' applicazione per la risoluzione di un problema reale legato alia bonifica in situ di amianto fioccato presente all'universita di Jussieu (Parigi, Francia). KEY WoR DS: Asbestos, chrysotile, grunerite, c01nbined Rietveld-RIR method, loose asbestos containing materials, epoxy resin.
2 2 A.F. GUALTIERI INTRODUCTION Asbestos minerals are classified in amphibole species (anthophyllite, grunerite or mnosite, riebeckite or crocidolite and tremolite) and serpentine species: lizardite (Rucklidge and Zussman, 1965), antigorite (Kunze, 1961 ), chrysotile (Whittaker, 1956), and carlosturanite (Mellini et al., 1985). Asbestos fibers have been utilised since antiquity: anthophyllite for example was used in pottery in Finland in 2500 B.C., clothes made of asbestos were described by Carlemagne in 800 A.D. and Marco Polo in 1250 A.D. (Liddell, 1991). Major industrial use of asbestos began in 1878 with mining of chrysotile in Quebec (Canada) followed by crocidolite mining in 1910 and amosite mining in 1916 in South Africa. After more than 30 years, toxicity of asbestos was recognised: Doll in 1995 in fact observed increased mortality from lung cancer in British asbestos workers (Bhandari and Dhariyal, 1990). In 1972, in USA it was established a Permissible Exposure Limit (PEL) for asbestos of 2.0 fibres/ml (f/ml) as an 8-hour-time-weighted average (TW A) and in 1986 PEL was reduced to 0.2 flml. Currently there is ongoing concern about the health risks associated with exposure to asbestos since exposure to asbestos fibres is associated with diseases like asbestosis, mesothelioma, lung cancer. Concerning the hazardous effects, it is well known that surface features and physical shape of the asbestos particles play a key role in the interaction with the organism cell interface (Hochella, 1993; Langer et al., 1972; Johan et al., 1976; Thomassin et al., 1976; Jurand et al., 1983). According to Hume and Rimstidt (1992) the dissolution reaction of chrysotile in the ph range of lung fluids is: Mg 3 Si205(0H)4 + 6H+ 3Mg H4Si04 + H20. From this, they predicted that a 1 11m diameter chrysotile fibre would completely dissolve in the human lung in 9.0(4.5) months. Therefore, because the onset of disease is generally long (20 years), at least the first step in disease generation should be relatively quickly (Hoc ell a, 1993; Pott, 1987). From epidemiological and in vivo studies, it is clear that crocidolite fibres have a remarkably longer lifetime in the lung tissue than chrysotile (Jones et al., 1989) and thus more pathogenic than chrysotile since they seem relatively chemically stable in lung-like environments (Harington, 1962; Kane, 1993; Stanton et al., 1981). In addition, amphibole asbestos is more hazardous than chrysotile because it contains iron. In fact, hydroxyls and super-oxide free radicals as generated by catalysis on fibre surfaces and the toxic hydroxyl radicals are generated in the presence of free oxygen. The mechanism involves the reduction of oxygen via the oxidation of iron on the mineral surface and the basic equation is (Fenton, 1984): H202 + Fe2 + OH + OH - + Fe 3 + Regarding the physical shape, the activity among the different fiber types increases with decreasing diameter and increasing fibre length (Ross et al., 1993). Stanton et al. (1981) postulated that the optimum morphology for the induction of intrapleural cancer is a diameter of m and a length >8 flm. Concerning the cytoxicity, a number of in vitro and in vivo studies were carried out in the past but still a general picture is not clearly drawn. Because macrophages are avidly phagocytic, mineral particles are rapidly internalised, and macrophages release a diverse array of products (inflammatory activity) into their extracellular environment and stimulate oxidant production (Nathan, 1987). Alternatively, macrophages and neutrophils produce a number of enzymes, oxidants, chemo-attractants and cytokines (particularly TNF-a) which may: a) deactivate minerals; b) activate cell defense mechanisms; c) cause cell injury and abnormal cell function of epithelial cells, fibroblasts, and mesothelial cells, that is, they can initiate or take part to the disease process (Fenton, 1984; Weitzmann and Graceffa, 1984). The need of a characterisation and accurate
3 The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials 3 quantitative analysis of asbestos containing materials is of key importance for a number of reasons: (a) classification of the material typology and definition of the hazardousness degree for the application of new restrictive laws imposed by the environmental agencies (Veblen and Wylie, 1993); (b) classification of the material typology for a proper plan of intervention and disposal; (c) understanding of the interaction asbestos-organism in biological studies. The application of the Rietveld method to poorly crystalline mixtures containing disordered phases such as chrysotile is not possible. The Rietveld method is successful for the extraction of quantitative data when the structure of the crystalline phases in the mixture is ordered or has a limited extent of disorder. The structure of chrysotile is described as a cylindrical lattice, and has a large density of structure disorder. This causes reflections along well defined crystallographic directions to be broadened. In such conditions, the integrated intensity of the modulated bands as simulated in the Rietveld-type refinements are underestimated with respect to the observed profiles, and therefore the value of the phase fraction obtained from the Rietveld refinement leads to an incorrect amount of chrysotile. Gualtieri and Artioli (1995) developed a reliable structure model for the disorder in chrysotile. Without such a model, the application of the Rietveld method (Rietveld, 1969; Bish and Post, 1993; Young, 1993) is not possible. However, the developed model cannot fully account for the broadening of the diffraction peaks and therefore an internal normalisation by RIR (Reference Intensity Ratio) (Davis et al., 1990) is required. The combined Rietveld-RIR method offers a number of advantages: (a) it is based on a rigorous model for the structure of chrysotile; (b) the profile-fitting technique allows control and evaluation of all microstructural, instrumental, and textural parameters of the sample, so that the proposed structure model can be adopted to chrysotiles with different degree of disorder; (c) the phase fractions extracted by the Rietveld refinements are rescaled on the basis of the absolute weight of corundum originally added to the mixture as an internal standard (internal renormalization); (d) the technique is of straightforward application and advantageous in terms of sample preparation and time requirements. Since 1994, large areas of the University of Jussieu in Paris have been evacuated because it was unambiguously discovered that the framework of the building is composed of an asbestos rich material. This paper reports the description of the characterisation of the asbestos rich material collected at the building of the University of Jussieu in Paris (France) and a possible plan of intervention for the treatment of the hazardous material in situ. METHODS Theoretical background and previous studies. Chrysotile is described in terms of a cylindrical lattice (Wicks and O'Hanley, 1988; Titulaer et al., 1993). The description of the structure symmetry in the various chrysotile types is rather complex due both to the curvature of the lattice and to the statistical stacking of the layers. Since there is no univocal model for the chrysotile structure and its polytypes, Gualtieri and Artioli ( 1995) developed a structure model capable to satisfactorily describe the diffraction effects in the powder spectrum. The model was developed using the powder diffraction spectrum of the well characterised chrysotile from Jeffrey Mine, Quebec Canada. The structure was refined in space group C2/m, and the effect of layer curvature was modelled by a broadening parameter on the crystallographic direction b. Fig. 1 (after Gualtieri and Artioli, 1995) shows the calibration curves of the expected versus observed chrysotile content using the results of the Rietveld refinement alone (a), and using the RIR corrected values (b). In both cases the samples having different matrix composition lie on the same curve, indicating that the matrix effects have been perfectly accounted for.
4 4 A.F. GUALTIERI expected chrysotile (wt0/o) Fig. 1 - The calibration curves of expected vs observed chrysotile content (wt%) for the reference mixtures: (a) using the weights from the Rietveld refinements. The empty triangles are the ternary mixtures CH 1-CH8; (b) using the weights from the Rietveld refinements and RIR-renormalization. The empty squares are the ternary mixtures CH1-CH8, the empty circles are the CH9 and CHlO multicomponent mixtures (After Gualtieri and Artioli, 1995). Materials and experiments. Two samples from the building of the University of Jussieu in Paris (France) were analysed. The specimen la be led PARIS 1 was sampled from a ceiling of the building; the sample labeled P ARIS2 was sampled from a wall of the building. The samples were considered representative of the construction material of the building. A qualitative investigation by X-ray powder diffraction revealed that the sample PARIS 1 is composed mainly of amorphous material (rock or slag wool) with minor amounts of serpentine asbestos (chrysotile), calcite and brucite. The sample P ARIS2 is as well composed mainly of amorphous material (rock or slag wool) with minor amounts of grunerite, calcite and quartz. For the quantitative analysis, the powders were added 1 O%wt NIST standard corundum to carry out the Rietveld-RIR. Data were collected using a Philips Bragg-Brentano diffractometer with a curved pirolitic graphite monochromator on the diffracted beam, in the range 5-l with steps of , 10 s/step, 0.5 divergence slit, 0.1 mm receiving slit, and 0.5 antiscatter slit. Data sets were refined by the Rietveld method using GSAS (Larson and von Dreele, 1999). In GSAS, the structure factors were calculated by using the formal atomic scattering factors. The background was successfully fitted with a Chebyshev function with 16 coefficients. The peak profiles were
5 The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials 5 t<) w 0 o X Ca Co + cts L[) theta X10E 2 sample class B Gr Co Q ea theta X10E 2 Fig. 2- The observed and calculated patterns, and difference curve of the refinement of samples PARIS I (a) and PARIS2 (b).
6 6 A.F. GUALTIERI modelled using a pseudo-voight function with one gaussian and one lorenzian coefficient. The lattice constants, the phase fraction, and coefficients corresponding to sample displacement and asymmetry were also refined. The total number of parameters refined at the same time in the last stages of the refinements for each pattern was 40. The SEM (Scanning Electron Microscopy) analysis of the sample was performed on specimens of ea. 0.7x0.7x0.7 cm mounted on an AI holder and fixed with an Ag paste. Dehydration was performed under an IR lamp for 15 min and coating was performed using Au. A Philips XL 40/604 automated instrument was utilised with a vacuum of ea. I0-7 torr. In order to give a statistical significance to the observations, 20 frames were collected for each specimen. Frames were collected using a beam size of 5 mm and an intensity of 25 k V. RESULTS AND DISCUSSION Fig. 2a and 2b show the observed (crosses), calculated (continuous line) and difference curve (bottom line) of the refined patterns. A good agreement between the calculated and observed patterns is evident at low angle as well as at high angle. The agreement factors for the Rietveld refinements are: Rwp=9% and x 2 =2.1 for PARIS! and Rwp= ll% and x 2 =3.1 for PARIS2, respectively. The results of the quantitative analysis of the two samples are reported in Table 1. Fig. 3 shows the raw samples from the wall (a) and ceiling (b) of the University. PARIS I is composed of an intergrowth of free glass fibers (slag wool) and asbestos fibers plus some grains of crystalline material (mainly calcite). PARIS2 is composed of amphibole asbestos fibres interdispersed in a matrix of glass fibres. Qualitatively fibres looking rigid and brittle are glassy wool, fibres which are rolled with an hair-like shape are asbestos fibres. As it was expected the content of asbestos phases is larger than the maximum amount allowed by law. Thus, the whole building was reasonably evacuated in 1994 and a drastic plan of intervention is demanded. Among the various solutions, the neutralisation of the asbestos containing material can be performed in situ by spraying an epoxy resin on walls and ceiling which is capable to penetrate and cement the fibres, preventing its dispersion in air. Such intervention was described in detail in Gualtieri (1998) and Gualtieri (1999). TABLE 1 Results of the quantitative analysis of the samples PARISJ and PARIS2. phase Parisl Paris 2 Chrysotile 6.3(6) Grunerite 9.5(9) Brucite 0.6(2) Calcite 6.7(5) 5.0(6) Quartz 0.5(2) Glass 86(1) 85(1)
7 The aid ofx-ray pmvder diffi action to the characterisation and treatment of asbestos containing materials = 5 I-'ll a b = 21-'m Fig. 3 - SEM image of the untreated specimen sampled at the University of Jussieu Paris. Sample (a) is PARIS l, sample (b) is PARIS2.
8 8 A.F. GUALTIERI a = 5 f..!m b = 1 f..! m Fig. 4 - SEM magnified images of PARIS 1 after the interaction with the epoxy resin at a different magnification showing a clear change in the microstructure of the material.
9 The aid of X-Ray powder diffraction to the characterisation and treatment of asbestos containing materials 9 As discussed by Harington (1962), hemolitic activity of chrysotile asbestos is blocked by chelators, particularly those with affinity for Mg. There are a number of groups that may modify the surface chemistry of chrysotile fibers to reduce they cytoxicity. Although the monoionic polymer polyvinyl-2-pyridine N oxide (PVPNO) does not passivate chrysotile, some ecidic, water soluble polymers, such as carboxymethylcellulose (CMC) are effective (Schnitzer, 1974). Brown et al. (1990) published a report in which they describe the modification of the surfaces of amosite fibers (mostly cummingtonite-grunerite) with octyldimethyl-chlorosilane (C8) or octadecylmethylchlorosilane (C18) through in vivo studies showing that fibers coated with C 18 chains were dramatically less active at producing tumors. Besides, Pott et al. ( 1989) reports that actinolite with 2-polyvinylpyridine N-oxide hydrogen bonded to its surface produced fewer mesotheliomas with a longer latency period than actinolite without polymer. For these reasons the utilisation of an epoxy resins should also benefit for the neutralisation of the surface activity of asbestos. The investigated specimen were treated by epoxy resin (see description in Gualtieri 1999) and observed by SEM after the treatment in order to put into evidence the differences in the morphology and microstructure of the materials before and after the interaction with the epoxy resin. Fig. 4a,b are magnified image of PARISl after the treatment with the epoxy resin. It is evident a change in the micro-structure of the material which is now a diphasic material where the fibres and the crystals are now cemented by the resin. Fibres are thus captured in a solid matrix which inhibits the dispersion in air medium. The same applies for sample PARIS2 (fig. 5) = 2 jlm Fig. 5 - SEM magnified images of PARIS2 after the interaction with the epoxy resin.
10 10 A.F. GUALTIERI It is possible to say that a proper in situ intervention using an epoxy resin modifies the nature of the asbestos containing materials which do not release free fibres in air and thus restore a safe environment to the scientific community of the University. A plan of intervention on an industrial scale has been proposed by AXSON Technologies, a France enterprise which produces the epoxy resin for the treatment. The purpose is still under discussion by the France Government. CONCLUSIONS In the present work we successfully applied the combined Rietveld-RIR for the quantification of chrysotile asbestos in bulk materials from the main building of the University of Jussieu (Paris, France). The addition of an internal standard (RIR) is necessary to overcome the matrix (glassy, clay, heterogeneous) effects and better account for the structural disorder of chrysotile. The importance of the study is paramount for either intervention plans and biological studies. It was demonstrated that a proper intervention in situ with an epoxy resin modifies the nature of the asbestos materials which do not release free fibres in air and thus restoring a safe environment. In the specific case, quantitative characterisation of the material is necessary for the development of the proper composition of the epoxy resin since composition is terms of viscosity and solvent addition is strictly dependent upon the mineralogical composition. ACKNOWLEDGEMENTS AXSON Technologies and ST AC Roofing srl are acknowledged for permission of making experimental data on the PARIS project available. Grants were obtained from Italian C.N.R. and M.U.R.S.T. REFERENCES BHANDARI, R.K. and DHARIYAL, K.D. (1990) Asbestos and associated health hazards, Central Building Res. Inst. Roorkee, Oxford and IBH Pub. Co. PVT. LTD New Delhi, 54 pp. BISH, L.B. and PosT, J.E. (1993) - Quantitative mineralogical analysis using the Rietveld fullpattern fitting method. Am. Min., 78, BROWN, R.C., CATHEW, P., HOSKINS, J.A., SARA, E., and SIMPSON, C.F. (1990) - Swface modification can affect the carcinogenicity of asbestos. Carcinogenesis, 11, DAVIS, B.L., KATH, R., and SPILDE, M. (1990) The reference Intensity ratio: Its measurenlent and significance. Powder Diff., 5, FENTON, H.J.H. (1984) - Oxidation of tartaric acid in presence of iron. J. Chem. Soc., 65, GUALTIERI A.F. and ARTIOLI G. (1995) - Quantitative determination of chrysotile asbestos in bulk materials by combined Rietveld and RIR methods, Powder Diffraction, 10(4), GUALTIERI A.F. (1998) - A solution to the asbestos problem: the in situ impregnation by an epoxy resin. Reunion «Le traitment de l'amiante in situ» Press Club de France, Paris, 29 giugno GUALTIERI A.F. (1999) -A solution for the full impregnation of asbestos: the use of an epoxy polymer resin, J. App. Polymer Science, submitted. HARINGTON, J.S. (1962) -Natural occurrence of oils containing 3,4-benzpyrene and related substances in asbestos. Nature, 193, HOCHELLA, M.F. (1993) - Surface chemistry, structure, and reactivity of hazardous mineral dusts. in Health effects of mineral dusts. G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am. 28, HUME, L.A., and RIMSTIDT, J.D. (1992) - The biodurability of chrysotile asbestos. Am. Min., 77, JOHAN, Z.A., GONI, J., SARCIA, C., BONNAUD, G., and BIGNON, J. (1976) - Influences de certains acides organiques sur la stabilite du reseau du chrysotile. 6th Cong. Int. Geoch. Organique Technip. Ed. Paris, JoNES, A.D., VINCENT, J.H., MciNTOSH, C., MACMILLAN, C.H., and ADDISON, J. (1989) - The effect of fiber durability on the hazard potential of inhaled chrysotile asbestos fibers. Exper. Path., 37, JURAND, M.C., BIGNON, J., SEBASTIEN, P., and GONI, J. (1983) - Leaching of chrysotile asbestos in human lungs. J. Colloid. Interf. Sci.», 95, 1-9. KANE, A.B. (1993) - Epidemiology and pathology of asbestos-related diseases, in Health effects of mineral dusts. G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am. 28, KUNZE, G. (1961) - Antigorit. Strukturtheoretische Grundlangen aun ihre praktische bedetung fiir die
11 The aid of X-Ray powder d(ffraction to the characterisation and treatment of asbestos containing materials 11 weiters serpentin-forschung, Fortschr. Min. 39, LANGER, A.M., RUBIN, l. B., SELIKOFF, I.J., and POOLEY, F.D. (1972)- Chemical characterization of asbestos baby cores by electron microprobe analysis. J. Hystochem. Cytochem., 20, LARSON A.C. and VON DREELE R.B. (1999) GSAS: General structure analysis system. Report LAUR Loa Alamos National Laboratory, NM 130 pp. LIDDELL, D. (1991) - Exposure to mineral fibers and human health: historical backgroud. In Mineral fibers and health, D. Liddell and K. Miller Eds. Boca Ratan CRC Press Florida Cap 1. MELLINI, M., FERRARIS, G. and COMPAGNONI, R. (1985) - Carlosturanite: HRTEM evidence of a polysomatic series including serpentine. Am. Min., 70, NATHAN, C.F. (1987) -Secretory products of macrophages. J. Clin. Invest., 79, POTT, F. (1987) - Problems in defining carcinogenic fibres. Ann. Occup. Hygiene», 31, PoTT, F., RoLLER, M., ZIEM, U., REIFFER, F.J., BELLMANN, B., ROSENBRUCH, M., and HUTH, F. (1989) - Carcinogenicity studies of natural and man-made fibers with the intraperitoneal test in rats. in Non occupational exposure to mineral fibers. Bignon, J. Ed. IARC Sci. Publ. No 90, Lyon France, RIETVELD, H.M. (1969) -A profile refinement for nuclear and magnetic structures. J. App. Cryst., 2, Ross, M., NOLAN R.P., LANGER, A.M., COOPER, W.C. (1993) -Health effects of mineral dusts other than asbestos. in «Health effects of mineral dusts». G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am., 28, pp RUCKLIDGE, J.C. and ZUSSMAN, J. (1965) -The crystal structure of the serpentine mineral lizardite Mg3Si205(0H)4, Acta Cryst., 19, SCHNITZER, R.J. (1974) -Modification of biological swface activity of particles. Environ. Health Oers., 9, STANTON, M.F., LAYARD, M., TEGERIS, A., MILLER, E., MAY, M., MORGAN, E., SMITH, A. (1981) - Relation of particle dimension to carcinogenicity of amphibole asbestos and other fibrous minerals. J. Nat'l Cancer Inst., 67, THOMASSIN, H., GONI, J., BAILLIF, P., TOURAY, J.C. (1976) -Etude par spectrometrie ESCA des premiers stades de la lixiviation du chrysotile en milieu acide organique. C. R. Acad. Sci. Paris, 283, TITULAER, M.K., VAN MILTEBURG, J.C., JANSEN, J.B., and GEus, J.W. (1993) - Characterization of tubular chrysotile by thermoporometry, nitrogen sorption, drifts and TEM. Clays and Clay Min., 4, VEBLEN, D.R. and WYLIE, A.G. (1993) - Mineralogy of amphiboles and 1:1 layer silicates. in Health effects of mineral dusts. G.D. Guthrie and B.T. Mossman eds. Min. Soc. of Am. 28, WEITZMAN, S.A., and GRACEFFA, P. (1984) Asbestos catalyzes hydroxyls and superoxide radicals generation from hydrogen peroxide. Arch. Biochem. Biophys., 228, WHITTAKER, E.J.W. (1956) -The structure of chrysotile. I!. Clinochrysotile. Acta Cryst., 9, WICKS, F.J., and O'HANLEY, D.S. (1988) - Serpentine minerals: structures and petrology. in Hydrous Phyllosilicates S.W. Bailey ed. Min. Soc. of Am. 19, YouNG, R.A. (1993). The Rietveld method. Oxford University Press, 235 pp.
ERZSÉBET TÓTH (Eötvös L. University, Budapest): ASBESTOS-RELATED DISEASES AND REGULATIONS Outline 1. History and legal definition (mineralogy + morphology) 2. The useful properties of asbestos, its success
Asbestos General information Key Points Fire Non flammable and non combustible under normal conditions Chemically inert under normal conditions. Resistant to most solvents, acids and alkalis In the event
Asbestos Presence in a Factory that Produced Asbestos-Containing Products Hana Fajkovi Department of Geology, Faculty of Science, University of Zagreb, Horvatovac 95, 10000 Zagreb, Croatia, e-mail: (email@example.com)
Update of the scientific evidence on asbestos and cancer Kurt Straif, MD MPH PhD International Agency for Research on Cancer Lyon, France World Health Organisation Asturias, 17 March 2011 The IARC Monographs
Analysis of Asbestos in Soil Hazel Davidson Technical Marketing Manager Diversity of asbestos materials Methods of analysis Problems and issues The way forward Types of asbestos: Chrysotile (white), Amosite
Ann. occup. llyy.. Vol.. Mos. I 4. pp. 4-4. 98. Primed in Great Bnlain. Inhaled Panicles V 0003 4878/8,004-OSO3.00/O Pergamon Press Lid. (' 98 British Occupational Hygiene Society. ASBESTOS FIBRES IN THE
Influence of Fiber Type, Size, and Number in Human Disease: Conclusions from Fiber Burden Analysis Andrew Churg, MD Department of Pathology University of British Columbia Vancouver, BC, Canada Techniques,
Scientific Update on Safe Use of Asbestos Robert P. Nolan, PhD International Environmental Research Foundation New York, New York www.ierfinc.org When We Talk about Asbestos What Do We Mean? Anthophyllite
United Nations Secretariat ST/SG/AC.10/C.3/2012/48 Distr.: General 11 April 2012 Original: English Committee of Experts on the Transport of Dangerous Goods and on the Globally Harmonized System of Classification
Cancer Risk Factors in Ontario Dusts and Fibres dusts ANd fibres risk factor/exposure Cancer The context where high risks were reported Magnitude of risk* Strength of evidence a Asbestos Larynx Occupational
STANDARDS Toxic and Hazardous Substances, Title 29 Code of Federal Regulations (CFR) Part 1910.1001, Subpart Z Asbestos 1. INTRODUCTION IWU has a responsibility to provide a safe environment for students,
Endereço eletrônico http://www.atsdr.cdc.gov/asbestos/asbestos_whatis.html Search Index Home Glossary Contact Us CONTENTS Asbestos What Is Asbestos? Polarized Light Microscopy Slide of Asbestos Fibers.
The British Occupational Hygiene Society Faculty of Occupational Hygiene INTERNATIONAL MODULE SYLLABUS W504 ASBESTOS AND OTHER FIBRES Aim: Learning Outcomes: This module enhances the student s knowledge
MATERIALS ANALYSIS QUANTITATIVE DETERMINATION OF COMMON TYPES OF ASBESTOS BY DIFFUSE REFLECTANCE FTIR Solutions for Your Analytical Business Markets and Applications Programs Solution Note Materials Author(s)
ASBESTOS Know what it is and how you can protect yourself environmental affairs Department: Environmental Affairs REPUBLIC OF SOUTH AFRICA 1 What is asbestos? The term asbestos designates a group of naturally
Page 1 of 6 skip navigational links This is an archive page. The links are no longer being updated. Statement by Gregory R. Wagner, M.D. Director, Division of Respiratory Disease Studies National Institute
A review of the WHO s document on the adverse health effects of exposure to asbestos and WHO's recommendations on the prevention of asbestos-related diseases D.M. Bernstein * The WHO s Programme on Occupational
Asbestos The term asbestiform describes a mineral habit characterized by long, thin, strong, flexible fibers equivalent to hairs or whiskers How long? Definition varies Modern Uses of Asbestos Asbestos
Course Specification Course Title Asbestos and Other Fibres Code W504 Level Foundation Intermediate Advanced Pre-requisites None Course Material Course manual available from OH learning.com Coordinating
The Administration of Norfolk Island SAFE DISPOSAL OF ASBESTOS AT THE WASTE MANAGEMENT CENTRE The purpose of this document is to provide guidance on the safe removal and disposal of asbestos and asbestos-containing
BE.104 Spring Evaluating Environmental Causes of Mesothelioma J. L. Sherley Outline: 1) Toxicological mechanisms and causation evaluations 2) An environetics case: Asbestos and Mesothelioma Toxicological
Asbestos and Mesothelioma in Ontario May 29, 2010 CARWH Conference: Worker Health in a Changing world of work Loraine Marrett, PhD Outline Part I: Asbestos & its uses Part II: Asbestos & cancer Part III:
Asbestos Awareness at the University of Toronto What is Asbestos? Asbestos is a general term given to a group of naturally occurring mineral silicates that are made up of long thin fibres. These fibrous
VERMICULITE IS NOT ASBESTOS There are no real causes for concern about health risks from vermiculite: a review of the mineralogy of vermiculite and its fundamental differences to asbestos explains why.
Science-Based Facts Relevant Health Issues 2015 For environmental occupational health safe and responsible use SCIENCE-BASED FACTS AND RELEVANT HEALTH ISSUES 2015 ON THE DIFFERENT ASBESTOS FIBER TYPES:
Introduction to X-Ray Powder Diffraction Data Analysis Center for Materials Science and Engineering at MIT http://prism.mit.edu/xray An X-ray diffraction pattern is a plot of the intensity of X-rays scattered
Asbestos Hazards and Controls Environmental and Occupational Health Public Health Ontario Photo provided with the kind permission of Infrastructure Health & Safety Association 5110 Creekbank Road, Mississauga,
National Institute of Standards & Technology Certificate Standard Reference Material 1866b Common Commercial Asbestos This standard reference material (SRM) is comprised of three commercial-grade asbestos
When worlds collide: Asbestos analysis in the regulatory, health, and mineralogical communities Heather Lowers and Gregory Meeker U.S. Department of the Interior U.S. Geological Survey What is a mineral?
Presence of Asbestos in Talc 1 The Presence of Asbestos in Talc Courtney Hardy Quantitative Methods in Rocks and Minerals Steven Teeter and Assistant Sandie Brundin July 17, 2010 Presence of Asbestos in
Health Effects of Asbestos Exposure Jill Dyken, PhD, PE John Wheeler, PhD, DABT Agency for Toxic Substances and Disease Registry Asbestos Science Seminar Folsom, California August 18-19, 2004 Agency for
Toxicity of Amphibole Asbestos Disclaimer: The material presented in these slides has been reviewed by the U.S. EPA and approved for presentation. Approval does not signify that the contents necessarily
Asbestos Prepared by: Penny Digby Principal Adviser (Occupational Health) Workplace Health and Safety Queensland Part 1. Overview types history respiratory system and defence mechanisms asbestos related
Industrial Health 2001, 39, 127 131 Original Article The Trend in Airborne Asbestos Concentrations at Plants Manufacturing Asbestos-Containing Products in Japan Koji YOSHIZUMI 1 *, Hajime HORI 2, Toshihiko
1 Risk Anal. 2004 Jun;24(3):547-52. Related Articles, Links Mesothelioma among brake mechanics: an expanded analysis of a casecontrol study. Hessel PA, Teta MJ, Goodman M, Lau E. Exponent, Wood Dale, IL
What is nanotoxicology? How to estimate the potential hazard related to nanoparticles? Dissemination report October 2008 DR-225 200810-5 Project ID NMP2-CT-2005-515843 An European Integrated Project Supported
The Management of Asbestos at the University of Manitoba WHAT IS ASBESTOS? Asbestos is a name given to a group of minerals which occur naturally as masses of long silky fibres. Asbestos is known for its
All About Asbestos Read this booklet to learn more about: identifying asbestos-containing material in you home the health risks of asbestos what you can do about asbestos. What Is Asbestos? Asbestos is
Frequently asked questions Asbestos investigation An investigation into asbestos-related health concerns has found that there is no evidence of elevated asbestos-related health risk to residents who have
Naturally Occurring Asbestos (NOA) General Overview Lee R. Shull PhD Health, Ecology and Risk Practice MWH Global Sacramento, CA CASH NOA Workshop January 24, 2006 Presentation Outline Brief background
C162 Asbestos Convention, 1986 Convention concerning Safety in the Use of Asbestos (Note: Date of coming into force: 16:06:1989.) Convention:C162 Place:Geneva Session of the Conference:72 Date of adoption:24:06:1986
Why TEM is essential in the measuring the concentration of airborne asbestos fibers Dr Maxime MISSERI THE AIRBORNE ASBESTOS FIBERS Six minerals that can divide into very thin fibers, have been recognized
All About Asbestos Read this booklet to learn more about: identifying asbestos-containing material in your home the health risks of asbestos what you can do about asbestos. What is Asbestos? Asbestos is
APPENDIX 1 NHS Barking and Dagenham Briefing on disease linked to Asbestos in Barking & Dagenham 1. Background 1.1. Asbestos Asbestos is a general name given to several naturally occurring fibrous minerals
Asbestos and Related Durable Fibers: Too Ubiquitous, Too Persistent, Too Complex to Put Health Risks to Rest? Philip M. Cook Mid-Continent Ecology Division National Health and Environmental Effects Research
A case study of performance degradation in insulating panels: Comparison between Blanket Aerogel and Mineral Wool Panels Francia Elena Prof. Siligardi Cristina Corso di Laurea Magistrale Ingegneria dei
June 2012 This fact sheet provides information to people who are trying to determine whether there is asbestos-containing material in their home or workplace, and what they might do if there is asbestos.
Mesothelioma Trends as Predictors of the Asbestos- Related Lung Cancer Burden Valerie McCormack UICC World Cancer Congress Montreal August 2012 Outline Background Estimating the lung cancer mortality burden
ASBESTOS AWARENESS Asbestos Awareness Asbestos is a serious health hazard commonly found in our environment today. This module is designed to provide initial education of asbestos and its associated hazards.
1 Asbestos Diseases What Is Asbestos? Asbestos is a term applied to a group of minerals formed into rock and mined in a similar way to coal. In this form, asbestos is made up of strong, fine and flexible
Asbestos and Mesothelioma a briefing document for the Metropolitan Police Prepared by Professor John Cherrie, Heriot Watt University, Edinburgh, UK. Introduction The purpose of this document is to provide
Elimination of Asbestos- Related Diseases WHO action Dr Ivan D. Ivanov Public Health and Environment WHO Headquarters Worldwide 125 million people are exposed to asbestos (mostly chrysotile) 75 million
Monitoring of Asbestos in urban and industrial environments of selected Italian sites. The case of a ceramic factory D. Mangano 1, A. F. Gualtieri 1, G. Torri 1, S. Ferrari 1, A. Ricchi 2, E. Foresti 3,
ASBESTOS AWARENESS at THE UNIVERSITY AT ALBANY University at Albany Office of Environmental Health and Safety 2010 Introduction - ASBESTOS WHAT IS IT? ASBESTOS is a fibrous material that occurs naturally
ASBESTOS IN SOIL AND MADE GROUND What is Asbestos? The word "asbestos" comes from the Greek meaning "inextinguishable." Asbestos is a serious health hazard commonly found in our environment today. Projects
Scanning Electron Microscopy Services for Pharmaceutical Manufacturers Author: Gary Brake, Marketing Manager Date: August 1, 2013 Analytical Testing Laboratory www.atl.semtechsolutions.com Scanning Electron
Call for an International Ban on Asbestos To eliminate the burden of disease and death that is caused worldwide by exposure to asbestos, The Collegium Ramazzini calls for an immediate ban on all mining
A Discussion of Asbestos Detection Techniques for Air and Soil August 2004 Prepared by Anthony Perry National Network of Environmental Management Studies Fellow for U.S. Environmental Protection Agency
RELATED TO EXPOSURE TO ASBESTOS AT WORK [S.L.424.23 1 SUBSIDIARY LEGISLATION 424.23 RELATED TO EXPOSURE TO ASBESTOS AT WORK REGULATIONS LEGAL NOTICE 323 of 2006. 15th December, 2006 1. (1) The title of
ASBESTOS AWARENESS For workers and building occupants Asbestos Awareness Asbestos is a serious health hazard commonly found in our environment today. This module is designed to provide an overview of asbestos
Naturally-Occurring Asbestos Information Asbestos is a term used for several types of naturally-occurring fibrous minerals found in many parts of California. The most common type of asbestos is chrysotile,
Asbestos - Frequently Asked Questions 1. What is asbestos? Asbestos is the name given to a group of fibrous minerals which occur naturally in the earth. These are grouped into two mineral types known as
Comments of Professor Richard Wilson Department of Physics & Center for Risk Analysis Harvard University Cambridge, Massachusetts On the Proposed Asbestos Ban Senate Employment and Workplace Safety Subcommittee
Facilities Operations and Development Environmental Health & Safety 1314 Kinnear Rd. Columbus, Ohio 43212 Phone (614) 292-1284 Fax (614) 292-6404 http://fod.osu.edu The Ohio State University Asbestos Management
EFFECT OF CHILDREN'S AGE AND LIFE EXPECTATION ON MESOTHELIOMA RISK 1 Robin Howie 2, Robin Howie Associates, Edinburgh It is generally accepted that the major risk from "low" level exposures to asbestos
Sir William Osler: Listen to the patient; the patient tells you everything. Jean-Martin Charcot: The patient is a liar. Epidemiology of Mesothelioma Jeffrey H. Mandel, MD, MPH Division of Environmental
Ingraham Environmental Inc. is committed to working with you to ensure that the environments where you live, work, and play are safe. We strive to provide you with the knowledge, experience and facts you
IUCLID 5 COMPOSITION AND ANALYSIS GUIDANCE DOCUMENT: IRON ORES, AGGLOMERATES [EINECS NUMBER 265 996 3, CAS NUMBER 65996 65 8] IRON ORE PELLETS INTRODUCTION Each REACH registrant is required to file its
MODELS FOR MESOTHELIOMA INCIDENCE FOLLOWING EXPOSURE TO FIBERS IN TERMS OF TIMING AND DURATION OF EXPOSURE AND THE BIOPERSISTENCE OF THE FIBERS G. Berry Department of Public Health and Community Medicine,
Kern, A., Madsen, I.C. and Scarlett, N.V.Y. This document was presented at PPXRD - Pharmaceutical Powder X-ray Diffraction Symposium Sponsored by The International Centre for Diffraction Data This presentation
DURABILITY OF MORTAR LININGS IN DUCTILE IRON PIPES Durability of mortar linings I. S. MELAND SINTEF Civil and Environmental Engineering, Cement and Concrete, Trondheim, Norway Durability of Building Materials
X-Ray Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye X-rays are electromagnetic radiation of wavelength about 1 Å (10-10 m), which is about the same size as an atom. The
No. 26705 MULTILATERAL Convention (No. 162) concerning safety in the use of asbestos. Adopted by the General Conference of the International Labour Organisation at its seventysecond session, Geneva, 24
Asbestos in the Home MISAWA AB, JAPAN Asbestos Awareness OCCUPANT ACKNOWLEDGEMENT OF INFORMATION SIGNATURE UNIT NUMBER DATE Prepared by: 35 CES/CEV If you have further question about location of asbestos
X-RAY DIFFRACTION PROCEDURES For Polycrystalline and Amorphous Materials HAROLD P. KLUG HEAD OF THE DEPARTMENT OF RESEARCH IN CHEMICAL PHYSICS LEROY E. ALEXANDER SENIOR FELLOW IN X-RAY DIFFRACTION Mellon
CARDIFF AND VALE NHS TRUST YMDDIRIEDOLAETH GIG CAERDYDD A R FRO Policy for the Management of Asbestos Author Keith Jones Estate Controls Assurance Officer / Environmental Management Co-ordinator Policy
Policy Asbestos Management Version 1.0 Adopted by Council at its meeting on 15 June 2010 Minute No: 390 Division: Planning and Regulation Section: Building and Health File Reference: Council Policies/Protocols/Procedures
ASBESTOS AWARENESS With details specific to The University of Alabama campus What is Asbestos It is the name given to 6 naturally occurring minerals mined from the earth. Crystalline structure forms long
THE MINISTRY OF ENVIRONMENTAL PROTECTION, PHYSICAL PLANNING AND CONSTRUCTION 1389 Pursuant to Article 104 paragraph 1 item 4 of the Waste Act (Official Gazette 178/04, 111/06), the Minister of Environmental
Brief X ray powder diffraction analysis tutorial Bibliografia essenziale X-ray powder diffraction (XRPD): un breve richiamo Analisi qualitativa Analisi quantitativa (metodo Rietveld) Dr Carlo Meneghini
Ann. Occup. Hyg., Vol. 52, No. 6, pp. 455 461, 2008 Ó The Author 2008. Published by Oxford University Press on behalf of the British Occupational Hygiene Society doi:10.1093/annhyg/men036 Asbestos Fibre
University of Nevada, Reno ASBESTOS AWARENESS TRAINING PROGRAM For workers and building occupants John A Braun, CSP Asbestos Awareness OSHA Standards for Asbestos are: 29 CFR 1910.1001 applies to all occupational
1 Asbestos as a metaphor for teaching risk perception (modified slightly from Gunter, M.E. (1994) Journal of Geological Education, 42, 17-24) ABSTRACT Asbestos -- the word means different things to different